Induced  smectic  ordering  and  blue  phase  formation  in  mixtures  of cyanobiphenyls and cholesterol esters

## Natalia  A.  Kasian a,b , Longin  N.  Lisetski a, *,  Serhii  E.  Ivanchenko c , Vitalii O. Chornous d , Halyna V. Bogatyryova e , Igor A. Gvozdovskyy e, **

a Department of Nanostructured Materials, Institute for Scintillation Materials of STC 'Institute  for  Single  Crystals'  of  the  National  Academy  of  Sciences  of  Ukraine, Kharkiv,  Ukraine; b Faculty  of  Physics,  Warsaw  University  of  Technology,  Warsaw, Poland; c Department  of Physical Chemistry and Technology of Nanostructured Ceramics and Nanocomposites, Frantsevich Institute for Problems of Materials Science of  the  National  Academy  of  Sciences  of  Ukraine,  Kyiv,  Ukraine; d Department  of Medical and Pharmaceutical Chemistry, Bukovinian State Medical University, Chernivtsi, Ukraine; d Department of Optical Quantum Electronics, Institute of Physics of the National Academy of Sciences of Ukraine, Kyiv, Ukraine;

Institute for Scintillation Materials of STC 'Institute for Single Crystals' of the National Academy of Sciences of Ukraine, 60 Nauky ave., 61072, Kharkiv, Ukraine, telephone number: +380 057 3410321, *E-mail: lcsciencefox@gmail.com

Institute of Physics of the National Academy of Sciences of Ukraine, 46 Nauky ave.,

Kyiv, 03028, Ukraine, telephone number: +380 44 5250862, ** E-mail: igvozd@gmail.com

It  has  been  found  that  in  mixtures  of  nematic  E7  and  smectogenic  cholesteryl oleyl carbonate (COC) the SA-N *  transition temperature is substantially (by ~20 K) increased, as compared with pure COC, at E7 concentrations around ~40%. Within  the  same  concentration  range,  the  isotropic  transition  is  preceded  by formation of blue phase, with its maximum width of ~3.5 K clearly correlated to the increased thermal stability of the SA phase. With other cholesterol esters or cyanobiphenyls (cholesteryl nonanoate, 5CB), this effect was either much weaker or  not  observed.  No  enhancement  of  smectic  phase  was  noted  when  E7  was replaced by Ntb-forming nematic mixture based on CB7CB with two cyanobiphenyl moieties. Selective Bragg reflection of light (BRL) spectra were measured  in  all  three  temperature  regions,  including  the  unwinding  of  the cholesteric  helix  on cooling  towards  SA phase  and  characteristic selective  BRL changes  in  the  blue  phase.  In  the  latter  case,  the  measured  λmax  values  were dependent both on the helical twisting power in the cholesteric phase and on the lattice size and orientation in the blue phase. Also considered were the effects of ferroelectric BaTiO3 nanoparticles accumulated at disclination lines upon the blue phase thermal stability.

Keywords: Induced smectic phase; nematic; chiral nematic; blue phases; nanoparticles; twist-bend nematic.

## 1. Introduction

Among  specific  phenomena  that  can  be  observed  in  multi-component  liquid  crystal systems,  one  of  the  most  intriguing  is  formation  of  induced  smectic  phases  (ISP)  in nematic  mixtures  comprising  components  of  different  chemical  nature.  In  this  case, certain  features  of  intermolecular  interactions  evoke  substantial  enhancement  of  the tendency  to  translational  ordering,  which  is  already  present  in  latent  form  in  the component molecules.

The  most  frequently  noted  mechanism  giving  rise  to  ISP  is  the  formation  of charge-transfer complexes, e.g. , between alkylcyanobiphenyls and azomethines (Schiff bases),  as  described  in  a  classical  work  of  Park  et  al.  [1]  However,  other  possible mechanisms were also proposed, together with a review of other pioneering works in this  field.  [2]  No  evidence  of  intermolecular  complex  formation  was  found  for  5CB doped with 4-pentylbenzoic acid system manifesting clearly expressed ISP properties; [3] on  the  other  hand,  formation  of  complexes  between  alkylcyanobiphenyl  and dialkylazoxybenzene  molecules  was  clearly  noted  even  in  isotropic  solvents.  [4]  A comprehensive review and analysis for various cases of ISP formation was presented in. [5] Since then, there has been not much attention to this topic. An attempt to develop a generalised  theoretical  model  describing  ISP  formation  caused  by  complexation  via specific interactions between two dissimilar molecules was made in. [6] Combining the Maier-Saupe theory for orientational ordering and McMillan theory for smectic layered ordering with the Flory-Huggins theory for isotropic mixing, the authors succeeded in deriving various types of phase diagrams observed in different systems. One can also mention detailed studies of the 4-n-octyl-4´-cyanobiphenyl (8CB) and 4,4´-di-n-heptylazobenzene (7AB7), forming a great variety of induced smectic phases upon mixing. [7]

As a more recent example, ISP was noted in mixtures of two nematogenic substances possessing low-temperature twist-bend phases (a cyanobiphenyl dimer and benzoyloxybenzylidene dimer) [8]. In this case, the mixtures showed no new absorption bands in the  wide  spectral  range,  implicating  the  absence  of  any  significant  charge  transfer  or even  dipole  -  induced  dipole  interaction.  The  smectic  arrangement  was  presumably promoted  by  geometrical factors, with intercalated structures of the constituent molecules providing the necessary driving force for ISP.

Another interesting case of ISP formation due to geometrical factors was noted in  [9].  In  the  mixtures  of  5CB  and  cholesteryl  oleyl  carbonate  (COC),  the  SA-N * transition temperature of COC was increased by about 3 K upon addition of 20 wt. % of 5CB, and returned to its initial value only at ~ 40 wt. % of 5CB. The explanation was given in terms of 5CB monomers or dimers (depending on 5CB concentration) aligning themselves between the stretched long hydrocarbon chains of adjacent COC molecules.

However,  no  less  intriguing  and  interesting  is  another  feature  that  can  be observed  in  highly  chiral  media,  namely,  the  formation  of  so-called  'blue  phases' (BPs),  which  are  thermodynamically  stable  within  a  narrow  temperature  range  ( e.g. about 1 °C, as experimentally found by Meiboom et al [10] for cholesteryl nonanoate (CN))  .The  existence  of  BPs  was  first  theoretically  explained  by  Brazovskii  et  al. [11,12] Later Meiboom et al [13] and Wright et al [14] have described, basing on the Oseen-Frank elasticity equations, an unstable planar texture of cholesterics (N ) near the * isotropic phase (Iso) characterised by a network of disclination lines of body-centered cubic ( i.e. BPI) or simple cubic ( i.e. BPII) lattice (as schematically shown in Figure 1 (a), (b) and Figure 1 (c), (d), respectively).

Figure 1. Schematic presentation of BPs characterised by: (a) simple cubic lattice for BPII and (c) body-centered cubic lattice for BPI formed by double-twist cylinders. BPs disclination  lines  are  shown  for  (b)  BPII  and  (d)  BPI.  Stabilisation  of  the  BPs  by nanoparticles is shown in (e) for BPII and (f) for BPI.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-2e25046f-67c0-4ceb-abd8-566dddb2de9f.jpg)

Blue  phases  as  highly  chiral  liquid  crystal  media  are  characterised  by  the presence of double-twist cylinders (Figure 1 (a), (c)) [14] and self-assembled into 3D photonic crystals showing selective BRL with relatively narrow spectrum. Due to this fact they have high potential of application in the manufacturing technology of displays, various kinds of sensors and photonic devices. [15-23] Such BP media are characterised by typical platelet textures [24] having domains with differently oriented lattice planes ( i.e. selective  BRL  colours)  observed  in  polarising  optical  microscope  (POM).  The lattice planes are characterised by Miller indices [ h , k , l ] ( h + k +   is an even number), l and the reflected light, according to Bragg's law, can be written as follows:

$$\lambda _ { _ { ( h k, l ) } } = \frac { 2 n \cdot a } { \sqrt { h ^ { 2 } + l ^ { 2 } + k ^ { 2 } } } \, \quad \, \quad \, ( 1 ),$$

where a is the lattice constant of BPs and n is refractive index.

Dierking  et  al  have  shown  in  [25,26]  that  experimentally  observed  platelet texture of BPs can be rather accurately recreated by using Voronoi diagrams. [27] The uniform  alignment  of  the  lattice planes by  using  different aligning layers ( e.g. numerically studied by Fukuda et al [28] and experimentally obtained by Glesson et al

[29],  Kikuchi et al [30] and Otón et al, [31]) and patterned surfaces, [32-34] leads to clearly  observed  diffraction  lines  under  the  reflective  POM  ( i.e. so-called  Kossel diagrams). [35,36] This is important for the use of BP  medium  for  different applications.

While high chirality of liquid-crystalline medium is main condition to form BPs, the  availability  of  network  of  the  lattices  is  even  more  important  condition.  This  is supported  by  formation  of  BPs  even  when  this  network  is  filled  by  non-chiral  ( e.g. nematic E7) liquid-crystalline medium, as shown by Xiang and Lavrentovich. [37] In addition, with series of non-chiral bent-core dimeric molecules recently discovered by Imrie  et  al,  [38]  chiral  liquid  crystalline  mediums  can  be  formed  having  smectic structure,  which in the  case  of chiral bent-core  molecules with cholesteryl group,  can additionally possess blue phases. [39,40]

The significant drawback of BPs, i.e. their narrow temperature range was largely overcome  by  adding  to  liquid-crystalline  medium  of  different  types  of  nanoparticles (NPs),  [41,42]  polymer  mesogens  to  form  polymer  networks  [43-45]  or  various molecules  having  different  shapes  ( e.g. bimesogenic,  [46]  T-shaped,  [47]  hydrogenbonded  [47-49]  and  non-chiral  bend-core  molecules  [38]).  In  addition,  it  should  be noted that the increase of stability of the BPs temperature range could be achieved using surface-functionalised graphene nanosheets - such effect was observed by Lavrič at al [50] even for minute concentrations of dispersed graphene.

In this manuscript the ISP formation in mixture based on nematic E7 doped with cholesteryl oleyl carbonate (COC) within wide concentration range from 0 to 100 wt. % was  studied.  It  has  been  shown  that  the  blue  phase  appeared  in  the  same  COC concentrations where the ISP was the most pronounced. Further temperature stabilisation  of  BP  was  achieved  by  adding  of  ferroelectric  nanoparticles  BaTiO3  as previous  described  in  detail  by  Wang  et  al.  [51]  In  addition,  alongside  E7-COC,  we studied  mixtures  of  COC  with  twist-bend  nematics  CB7CB/CB6OCB/5CB  in  ratio (39:19:42) under similar experimental conditions. Also, in parallel series of experiments we used cholesteryl nonanoate (CN) as another example of smectic-forming cholesterol esters. As compared to COC, its hydrocarbon chain is saturated and much shorter.

## 2. Materials and methods

## 2.1 Materials

To  study  the  induced  smectic  phase  the  nematic  liquid  crystals  mixture  E7,  which contains cyanobiphenyl and cyanoterphenyl components, was obtained from Licrystal, Merck (Darmstadt,  Germany).  It  was  chosen  because  its  temperature  of  the  nematicisotropic transition is higher ( i.e. T Iso is 58 ºC [52]) than for recently described mixtures on the base of the nematic 5CB. [9] As another type of the nematic liquid crystalline medium to form the ISP, we used a three-component mixture consisting of two achiral liquid crystal dimers, i.e. 1'-,7"-bis-4-(4-cyanobiphen-4'-yl)heptane (CB7CB) and 1-(4cyanobiphenyl-4'-yloxy)-6-(4-cyanobiphenyl-4'-yl)hexane (CB6OCB), and the monomer nematic  4-pentyl-4'-cyanobiphenyl  (5CB)  (Figure  2  (a),  (b),  (c))  in  weight ratio (39:19:42), which was recently used to prepare N * tb -forming system possessing the oblique helicoidal structure. [53,54] The twist-bend nematic CB7CB was synthesised in Bukovinian  State  Medical  University  (Chernivtsi,  Ukraine)  with  its  characteristics described in detail. [55] The N phase of synthesised CB7CB is observed for temperature range  from  103  to  116  °C.  The  twist-bend  nematic  CB6OCB  was  obtained  from Synthon  Chemicals  GmbH  &amp;  Co  (Wolfen,  Germany),  and  possesses  N  phase  within temperature range  from  109 to 157 ºC. [55-57]  The nematic 5CB was synthesised in STC 'Institute of Single Crystals' (Kharkiv, Ukraine) and purified before using.

Figure  2.  Chemical  structures  of  compounds  used.  The  twist-bend  nematic-forming mixture  consists of: (a) -39 wt. %  of  1'-,7"-bis-4-(4-cyanobiphen-4'-yl)heptane (CB7CB),  (b)  -  19  wt.  %  of  1-(4-cyanobiphenyl-4'-yloxy)-6-(4-cyanobiphenyl-4'yl)hexane  (CB6OCB)  and  (c)  -  42  wt.  %  of  4-pentyl-4'-cyanobiphenyl  (5CB).  The

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-89b36aae-8c69-4719-9c9f-20ee82a06976.jpg)

cholesterol esters as chiral compounds: (d) - cholesteryl oleyl carbonate (COC) and (e) cholesteryl nonanoate (CN).

The cholesteryl oleyl carbonate (COC) (Figure 2 (d)) as chiral dopant (ChD) was obtained from Aldrich (USA).  COC  possesses  various liquid-crystalline phases, including smectic A phase (SA), the temperatures of phases transitions and their ranges were presented in detail by Lebovka at al. [9]

The cholesteryl nonanoate (CN) (Figure 2 (e)) was synthesised in A.V. Bogatsky Physico-Chemical  Institute  of  the  NAS  of  Ukraine  (Odesa,  Ukraine).  By  taking  into account the fact that for CN the SA phase is also observed [58,59], we also used this substance for a comparative study.

The concentration of ChDs in the nematic host E7 for both the COC and the CN was  changed  in  range  from  0  to  100  wt.  %.  The  concentration  of  ChDs  in  ISP  was changed with the step about 5 wt. %.

To  stabilise  BPs  of  COC-containing  mixtures,  we  added  ferroelectric  BaTiO3 NPs synthesized in Frantsevich Institute for Problems of Materials Science of the NAS of Ukraine (Kyiv, Ukraine). The size of NPs with an average diameter of approximately 24  nm  was  achieved.  The  NPs  were  covered  by  oleic  acid  and  further  dissolved  in heptane to create uniformed suspension. This suspension was mixed with LC mixture, containing the chiral dopant COC and nematic E7 in different weight ratio. The detailed description of preparation of ferroelectric NPs is given in the section Methods.

To obtain planar alignment of various studied mixtures ( i.e. N * and N * tb -forming mixtures)  polyimide  PI2555  (HD  MicroSystems,  USA),  [60]  known  for  its  strong azimuthal anchoring energy, [61] was used.

## 2.2 Methods

The  glass  substrates  (microscope  slides,  made  in  Germany)  were  covered  with  nmenthyl-2-pyrrolidone solution of PI2555 in ratio 10:1 and spin-coated (6800 rpm over 10 s) to obtain a thin alignment film. The substrates were dried at 80 °C for 15 min, and subsequent  thermopolymerisation  of  polyimide  molecules  at  180  °C  was  carried  out during 30 min. The PI2555 film was rubbed Nrubb = 15 times to ensure strong azimuthal anchoring energy about 10 -5 J/m . [61] 2

LC cells were assembled of two rubbed substrates oriented in such  a way that each of them had opposite rubbing direction with respect to another. The thickness of LC cell, set by spherical spacer of 20 µm diameter, was 21 ± 0.5 µm. The thickness was measured by interference method by recording of transmission spectrum of the empty LC  cell using an Ocean Optics USB4000  spectrometer (Ocean Insight, USA, California).

The chiral mixtures were prepared within wide concentration ratio of ChDs in host liquid-crystalline medium ( i.e. N, Ntb-forming mixture) from 0 to 100 wt. % with the minimum step about 5 wt. %. To create the uniform chiral mixtures, a Fisher Vortex Genie 2 mixer (Fisher Scientific, USA) was used with periodically heating the mixture to Iso (vortex 4-5 over 30 min). The LC cell was filled by using the capillary method at the  temperature  just  above  the  isotropic  transition  of  chiral  mixtures  to  avoid  the additional aligning of LC owing to the flow.

To stabilise the temperature range of BPs, as was described in detail elsewhere, [51]  we  used  the  ferroelectric  nanosized  barium  titanate  (BaTiO3)  powder  mainly consisting of NPs with ~ 24 nm in diameter. The NPs of BaTiO3 were synthesised using the  non-isothermal  decomposition  method  of  high-purity  barium  titanyl  oxalate, i.e. Ba(TiO)(C2O4)2, produced by Degussa Electronic Corporation (Netherlands). The nonisothermal decomposition of barium titanyl oxalate was carried out in a rotary furnace with 14 temperature zones, developed at Frantsevich Institute for Problems of Materials Science of the NAS of Ukraine (Kyiv, Ukraine), at temperatures within 650 - 700 °C.

To prepare the dispersion, BaTiO3 nanopowder (Nanotechcenter LLC, Ukraine) with  a  mean  particle  diameter  of  24  nm  was  used.  The  powder  was  submerged  in heptane  (Heltermann  Carless,  Germany)  with  the  addition  of  oleic  acid  (Heltermann Carless,  Germany)  at  a  mass  ratio  of  1:1.8:13.3,  respectively.  The  dispersion  was ground in a 50 ml glass jar with zirconia oxide balls for 48 hours on a rotary mill at a speed of 100 rpm.

The liquid-crystalline suspensions were prepared by doping of the LC mixture ( e.g. COC-E7 mixture containing 72.5 wt. % of COC and 27.5 wt. % of E7 or CN-E7 mixture  containing  62.3  wt.  %  of  CN  and  31.7  wt.  %  of  E7)  by  BaTiO3  NPs  within range  from  0.25  to  4  wt.  %.  The  subsequent  30  min  sonication  of  the  suspension  at temperature  of  BP-I  was  carried  out  by  means  of  the  UZDN-2T  ultrasonic  disperser (Ukrrospribor, Sumy, Ukraine), at the frequency of 22 kHz and the output power of 75 W.

To  measure  the  phase  transition  temperatures  of  studied  mixtures,  we  used  a thermostable heater based on a temperature regulator MikRa 603 (LLD 'MikRa', Kyiv, Ukraine) additionally equipped with a platinum resistance thermometer Pt1000 (PJSC 'TERA', Chernihiv,  Ukraine).  The  temperature  measurement  accuracy  was  ±  0.1 o C. During the BPs phase transition studies the speed of temperature change was about 0.01 o C/min (0.1  C per 10 min) both on heating and cooling. o

## 3. Results and discussions

3.1. Experimental study of induced smectic phase mixtures based on cholesteryl oleyl carbonate and nematic E7

This section will be  a certain continuation of studies  of the induced smectic phase in systems based on non-smectogenic nematic 5CB and cholesteryl oleyl carbonate (COC) recently described in detail by Lebovka at al. [9] Two important features were noted for these  mixtures,  namely  first  of  all,  the  increase  of  temperature  of  the  cholesteric  to smectic A (SA) transition induced in COC by addition of up to 20 wt. % of 5CB and secondly,  the  linear  dependence  of  reciprocal  helix  pitch  1/ P on  concentration  of nematic 5CB, as distinct from the most cases of nematic-cholesteric mixtures. However, the use of nematic 5CB to study all the concentration range from 0 to 100 wt. % in this ISP mixture is somewhat limited due to the low temperature of the Iso-N transition ( T Iso = 35.5 °C).

To  increase  the  concentration  range  of  the  non-smectogenic  nematic  in  ISP mixture in this work we propose to use the nematic characterised by higher temperature of Iso-N transition, for instance, the nematic E7 ( T Iso = 58 ºC [52]) which includes 51 wt. % of 5CB.

The phase transitions temperatures of the ISP mixtures, based on nematic E7 and certain concentration C COC of smectogenic chiral dopant COC, which lies in the range of 0 - 100 wt. %, are shown for both on heating (Figure 3a) and on cooling (Figure 3b). The Figure 3 also shows that during heating and cooling process the certain hysteresis is observed.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-b121e47a-800a-4d3f-ae64-02e3a12225f3.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-a2f8ef12-e9f9-47e7-af08-62ebedb1a6a8.jpg)

Gcoc'

Gcoc'

Figure 3. Dependence of temperatures of the phase transitions of ISP mixtures, based on COC and E7, on concentration C COC of the chiral dopant COC during: (a) heating (solid symbols)  and  (b)  cooling  (opened  symbols)  processes.  During  heating  process  the sequential  phase  transitions  of  the  E7-COC  mixtures  are  the  next:  SA  -  N   (solid * magenta circles), N  - Iso (solid black squares), N  - BPs (solid blue triangles), and BPs * * -Iso  (solid  black  squares).  During  cooling  process  the  sequential  phase  transitions  of ISP mixtures are the next: Iso - N  (opened black squares), Iso - BPs (opened black * squares), BPs - N  (opened blue triangles), N  - SA (opened magenta circles). The linear * * approximation for the N  - Iso transition during both heating and cooling is shown by * solid red line.

Figure 4 shows sequential change of textures of phase transitions of ISP mixture, e.g ., having COC concentration C COC = 72.5 wt. %, during cooling process. As can be seen  from  Figure  3b  this  ISP  mixture  is  characterised  by  all  phases  inherent  in  it, including BPs, N  and SA.[62] *

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-8139abb4-9e54-4485-8629-a989106abbdd.jpg)

Figure 4. Texture of ISP mixture, containing 72.5 wt. % of COC and 27.5 wt. % of nematic E7 on cooling: (a) Iso at 45.6 °C; (b) Iso - BPIII transition at 44.4 °C; (c) BPII characterised by simple cubic lattice at 44.2 °C; (d) BPI characterised by bodycentered cubic lattice at 42.5 °C; (e) BPI - N  transition at 45.6 °C; (f) N  phase at * * 38.4 °C, characterised helicoidal structure, with Grandjean-Cano ' planar ' texture and oily  streaks  defects;  (g)  N   -  SA  transition  at  36.3  °C  and  (h)  SA  phase  at  35.2  °C. * Thickness of LC cell was 26.1 µm. LC cell was placed between crossed polariser (P) and analyser (A). The rubbing direction of PI2555 layers was coincided with direction of polariser (P).

The certain deviation from linear dependence of temperature Iso-N  transition on * concentration of COC is observed (Figure 3) as was described in detail elsewhere [9] for ISP mixture, based on COC and 5CB. For the mixtures COC and E7 at concentrations of COC within range from 50 to 75 wt. %, the deviation is noted during both the heating and  cooling  processes  (Figure  3).  It  can  also  be  seen  that  at  these  concentrations  the region of blue phases appears additionally in ISP mixtures. It is interesting that t in this range of concentrations the temperatures of the SA - N  transitions (magenta circles) are * the highest and show only minor variation with temperature (within about 35 - 37 °C). Thus, it appears that there is a certain correlation and probably a relationship between the  induction  of  translational  order  and  formation  of  the  blue  phase.  This  will  be discussed in detail in our further narration.

The maximum of wavelength λmax of selective BRL in visible range of spectrum as  function  of  temperature T for  the  ISP,  consisting  of  72.5  wt.  %  of  COC  in  E7,  is shown in Figure 5. The red shift of λmax of selective BRL occurs during cooling of N . * For  this  ISP  mixture  N   possesses  sufficient  shift  of  wavelength  ( * i.e. about  120  nm) when the temperature changes within small range from 36 to 39 °C. This temperature range  refers  to  the  human  body  temperature,  including  both  the  normal  and  high temperature, and can be proposed for biomedical applications using the same ideology as, e.g. , in Ref. [63]

Figure 5. Transmission spectra of the N  containing 72.5 wt. % of COC and 27.5 wt. % * of  E7  at  different  temperatures:  1)  -  38.5  °C  (black  spectrum);  2)  -  37.3  °C  (red spectrum); 3) - 36.8 °C (green spectrum); 4) - 36.5 °C (blue spectrum); 5) - 36.2 °C (cyan spectrum) and 6) - 36.1 °C (magenta spectrum). Thickness of LC cell was 26.1 µm.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-ded1e509-8bc5-4cd9-af8f-5bea203d37f8.jpg)

Figure 6 shows the dependencies of reciprocal helix pitch 1/ P on temperature T in  the  case  when  ISP mixture containing a certain concentration of COC  is in the N * phase. The decrease of temperature T leads to the red shift of maximum wavelength of the selective BRL in the visible range, i.e. increasing of the pitch length P of helix in the N * phase.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-989f9c45-1ac8-4682-bc65-95a2695b8b96.jpg)

Figure  6.  Dependence  of  reciprocal  helix  pitch  1/ P on  temperature T ISP  mixture, containing certain concentration of COC, namely: 1) 14.3 wt. % (solid brown squares), 2) - 23.3 wt. % (solid dark cyan circles), 3) - 32.4 wt. % (solid royal triangles up), 4) 40.8 wt. % (solid magenta triangles down), 5) - 50.0 wt. % (solid purple diamonds), 6) - 61 wt. % (solid black triangles left), 7) - 65.1 wt. % (solid blue triangles right), 8) 70 wt. % (solid red pentagons), 9) - 72.5 wt. % (opened brown squares), 10) - 75.5 wt. % (opened green circles), 11) - 80.8 wt. % (opened blue triangles up), 12) - 84.6 wt. % (opened magenta diamonds), 13) - 90.0 wt. % (opened dark yellow triangles right), 14) - 95 wt. % (opened red pentagons), 15 - 100 wt. % (opened dark triangles down).

## 3.2  Blue  phases  of  induced  smectic  phase  mixtures  based  on  cholesteryl  oleyl carbonate and nematic E7

In  this  section  we  will  consider  the  ISP  mixtures  possessing  BPs.  As  was mentioned above, the BP is observed within concentration range of COC about 50 - 75 wt. %, where the deviation from linear dependence of T Iso (C) is observed (Figure 3).

The  textures  of  sequential  BPs  transitions  during  cooling  of  ISP  mixture, consisting 72.5 wt. % of COC and 27.5 wt. % of nematic E7, are shown in Figure 4 (b) (e).

Typically, in contrast to the process of heating (Figure 7(a)) during cooling the temperature ranges of BPs of ISP mixtures were wider (Figure 7(b)).

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-c500053c-7acc-4959-ab7e-1ce3ddeec4ed.jpg)

Figure 7. Temperatures of phase transitions of BPs of ISP-forming mixtures E7-COC within COC concentration range from 50 to 75 wt. % on heating (a) and cooling (b).

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-f90d41c1-f61f-4059-b3e6-04f6bf06fc50.jpg)

The transmittance spectrum of one of these BP-forming mixtures (72.5% COC and 27.5% E7) at different temperatures is shown in Figure 8. During cooling from Iso (black spectrum 1) the appearance of the BPIII (red spectrum 2), so-called fog phase, is observed.  Further  cooling  process  leads  to  sequential  appearance  of  BPII  (green spectrum  3)  and  supercooled  BPI  (blue  spectrum  4),  characterised  by  simple  cubic (Figure 2 (b)) and body-centered cubic (Figure 2 (c)) lattices, [62] respectively.

Figure 8. Transmission spectra of the BPs of IPS mixture containing 72.5 wt. % of COC and 27.5 wt. % of E7 at different temperatures during cooling: 1) - Iso at 45.4 °C (black spectrum); 2) - BPIII ( i.e. fog phase) at 44.4 °C (red spectrum); 3) - BPII at 43.9 °C (green spectrum); 4) - BPI at 42.5 °C (blue spectrum). Thickness of LC cell was 26.1 µm.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-0cf9a2ed-015e-43de-a77c-cba95c599010.jpg)

The use of ISP mixtures that are additionally characterised by BPs allows us to experimentally observe both continuous changes of maximum wavelength BRL of the N * at low  temperatures  (Figure  5)  and  the  discontinuous  changes  of  maximum wavelength BRL of the BPs at high temperatures of mixture (Figure 8).

Because  the  temperature  range  of  BPs  is  narrow  (Figure  7  (b)),  then  small temperature  changes  lead  to  the  sufficient  discontinuous  shift  ( i.e. about  100  nm)  of maximum of the selective BRL wavelength λmax, as can be seen in Figure 8. The main reason of discontinuous shift is the presence of the lattice for BPs. The selective BRL is described by  Equation  (1), which  relates the selective reflection wavelength  to characteristics  of  the  lattice  plane  with  indices  of  Miller  (h,l,k).  The  relationship between  the  length  of  cholesteric  helix P ( i.e. (  ) 1 ~ -C P ,  where  and C is  the helical twisting power of ChD and its concentration, respectively [62]) and BPs lattice size a for  the  first  time  was  experimentally  considered  by  Otón  et  al.,  [64]  and  our results seem to be in a qualitative agreement with their data.

## 3.3. Experimental study of induced smectic phase mixtures based on cholesteryl nonanoate and nematic E7

Our next step was to check whether the rather unusual behavior of correlated appearance of ISP and BPs in the E7-COC system would be observed for other chiral dopants forming SA.

In  this  section  we  will  consider  the  mixtures  of  E7  and  cholesteryl  nonanoate (CN). It is known that CN possesses sequential phases transitions, namely under heating Cr 75 °C SA 78.6°C N * 91.2°C Iso. [59] It should be noted that cholesterol esters from C9  to  C14  and  some  of  their  mixtures  were  studied  by  Duarte  et  al,  [65]  paying attention  to  density  measurements  during  first  and  second  order  SA  -  N   phase * transitions.

Figure 9 shows, both on heating and cooling, the phase transition temperatures for  various  mixtures  based  on  nematic  E7  and  CN  possessing  the  SA  phase.  [58,59] Typically, certain small hysteresis of the temperatures during the process of heating and cooling is observed.

Figure  9.  Dependence  of  temperatures  of  the  phase  transitions  of  E7-CN  systems  on concentration C CN of the chiral dopant CN during: (a) heating (solid symbols) and (b) cooling  (opened  symbols)  processes.  During  heating  process  the  sequential  phase transitions of the E7-CN mixtures are: SA - N  (solid green circles), N  - Iso (solid black * *

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-bfdfe6c1-e580-4a74-8f5b-78f56d7fe657.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-0a37b639-e80e-4f67-bffe-4b43de5df3cf.jpg)

squares),  N   -  BPs  (solid  red  triangles),  and  BPs  -  Iso  (solid  blue  squares).  During * cooling process the sequential phase transitions of ISP mixtures are: Iso - N  (opened * black squares), Iso - BPs (opened blue squares), BPs - N  (opened red triangles), N  -* * SA (opened green circles). The linear approximation for the N  - Iso transition during * both the process of heating and the cooling is shown by solid magenta line.

As in the case of E7-COC mixtures, the sequential phase transitions including SA, N * , BP and Iso are also observed. The temperatures of SA - N , N  - BP and BPs -* * Iso transitions are monotonically increasing with the increase of concentration C CN of CN. The dependence of temperature of phase transition on concentration of CN for the Iso (black symbols) has certain deviation from linear function (solid magenta line). This deviation is observed for the ISPs that are characterised by the appearance of BPs.  In contrary  to  ISP  mixtures  based  on  COC  (Figure  3)  the  appearance  of  BPs  for  CNcontaining  mixtures  within  concentration  range  from  40  to  80  wt.  %  leads  to  the decrease of temperature under BP - Iso transition (Figure 9). But the main difference between E7-COC and E7-CN systems is that the latter are, in fact, not ISP systems only a slight positive deviation from linearity of the  SA - N * transition  temperature is observed. This is accompanied by the fact that for the E7-CN system the observed BPs are noticeably narrower.

The  E7-COC  mixtures  are  characterised  by their rather pronounced  ISP mesomorphism, which for E7-CN is extremely weak. The most probable reason is that ISP  with  COC  is  due  to  steric  interactions  between  molecules  of  cyanobiphehyl  and cholesteryl oleyl carbonate with is very long hydrocarbon chain - this allows a certain equilibrium  between  cyanobiphenyl  dimers  and  cyanobiphenyl  monomers  arranged between the tails of adjacent COC molecules (as discussed in detail in [9]). Too short alkyl chains of cholesteryl nonanoate do not allow such arrangement, and ISP formation is not observed.

Also,  for  mixtures,  the  obtained  result  is  in  good  agreement  with  the  density measurements of first and second order phase transitions of cholesterol esters and their mixtures that are characterised by both SA and BPs. [65]

Finally, one can make an assumption that the observed correlation between ISP and BP formation can be explained by the short-range translational ordering above the SA  -  N   transition,  which  could  stimulate  the  lattice  formation  close  to  the  isotropic * transition.

## 3.4. ISP mixtures possessing stabilised BPs by means of BaTiO3 NPs

It  is  well  known  that  the  adding  of  NPs  to  BPs  leads  to  extension  of  the temperature interval of their existence. The main reason of stabilisation of BPs is that NPs  can  fill  space  in  disclinations  of  lattice  of  the  BPs,  as  schematically  shown  in Figure 2 (e), (f).

In  this  section  we  will  consider  the  temperatures  of  phase  transitions  of  ISP mixtures  with  blue  phases  stabilised  by  small  concentration  of  ferroelectric  barium titanate (BaTiO3) NPs. The main purpose of these studies is to find out the effects of NPs  used  to  stabilise  BPs  upon  changes  in  the  temperatures  of  phase  transitions, especially  BP-Iso  transitions  for  which  certain  deviations  from  linear  dependence  are observed (Figure 3).

It  should  be  noted  that  NPs  of  ferroelectric  BaTiO3  was  previously  used  for stabilisation of BPs of the mixture containing two chiral compounds, namely R-811 and Iso-(6OBA)2, and the nematic SLC-X. [51]

Figure  10  (a)  shows  the  dependence  of  phase  transition  temperatures  on concentration  of  BaTiO3  NPs  for  the  mixtures  that  are  characterised  by  the  wider temperature range of BPs, e.g. 72.5 wt.% COC and 27.5 wt.% E7, as can be seen from Figure  3  (b)  and  Figure  7  (b).  The  adding  of  the  NPs  leads  to  extension  of  the temperature range of the BPs.

Thus, for ISP mixture containing BaTiO3 NPs within certain concentration range from 0.5 to 1 wt. % the maximal broadening of the temperature range of existence of the BPs  was  observed  (Figure  10  (b)).  For  this  concentration  range  a  small  increase  in temperature  Iso  (solid  black  squares,  curve  1,  Figure  10  (a))  that  is  typical  for stabilisation  of  BPs;  in  particular,  this  applies  to  BaTiO3  NPs  described  in  detail elsewhere. [51]

The Figure 10 (a) shows that the increase of NPs concentration to 4 wt. % of BaTiO3 leads to the decrease of temperature Iso - BPs transition to the value as it is observed for the BPs without adding of NPs.  However, the significant  broadening of temperature range of BPs due to decrease of temperature transition BPs - N  (solid blue * circles, curve 2) is observed.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-ce4dc444-c49d-43ca-929a-9ae401488033.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-fae97895-8438-4946-91a7-937b957644c0.jpg)

Gcoc'

Figure 10. Dependence of the (a) temperature of phase transitions and (b) temperature difference between Iso and BPs during cooling for the ISP mixture consisting of 72.5 wt. % of COC and 27.5 wt. % of nematic E7 on concentration of BaTiO3 NPs.

According  to  the  data  shown  in  Figure  10,  we  can  assume  that  maximal influence on the deviation from linear dependence under phase transition to Iso should be observed when the presence of the 0.5 wt. % of BaTiO3 NPs in the ISP mixtures having  BPs.  However,  this  deviation  will  be  non  significant,  because  the  adding  of BaTiO3 NPs leads to a small increase of the temperature of the BPs - Iso transition.

Figure 11 shows the dependence of the temperature for Iso - BPs (black squares symbols)  and  BPs  -  N   (blue  circles  symbols)  transitions  of  ISP  mixtures  containing * certain concentration ratio between COC and E7 and additionally doped by 0.5 wt. % of BaTiO3 NPs, on the COC concentration.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-0dd93e95-3171-48bf-b31e-452a734ba306.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-57f39045-aa4d-4f60-a275-22df0f315cf1.jpg)

Ccoc'

Ccoc'

Figure  11.  Dependence  of  the  Iso  -  BP  (black  squares  symbols)  and  BP  -  N   (blue * circles symbols) phase transition temperatures in the studied ISP mixtures on concentration of COC during (a) heating (b) and cooling. The E7-COC ISP mixtures

were  additionally  doped  by  0.5  wt.  %  BaTiO3  NPs.  The  linear  dependence T C ( )  is shown by solid red line.

By  comparing  Figure  11  and  Figure  3  it  is  clearly  seen  that  the  presence  of BaTiO3  NPs  in  BPs  leads  to  increased  deviation  from  linear  dependence  of  Iso transition  ( i.e. ,  on  other  words,  the  pronounced  convexity).  In  addition,  BaTiO3  NPs stabilise BPs, so we can see the minimum hysteresis during heating (Figure 11 (a)) and cooling (Figure 11 (b)), in comparison with the ISP mixtures without NPs (Figure 3).

The adding of BaTiO3 NPs to mixtures containing CN and E7 leads to minor stabilisation  of  BPs,  in  comparison  with  ISP  mixtures  based  on  COC  and  E7  (Figure 10).  Figure  12  (a)  shows  the  phase  transition  temperatures  of  the  mixture  containing 62.3 wt. % of CN and 31.7 wt. % of nematic E7 as function of concentration of BaTiO3 NPs.  The  maximum  broadening  of  BPs  is  observed  upon  adding  of  NPs  within concentration range from 0.3 to 1.2 wt. %.

Figure 12. Dependence of the (a) temperature of  Iso - BPs (solid black squares) and BPs - N * (solid blue circles) transitions and (b) temperature difference between Iso and BPs (solid red spheres) during cooling for the E7-CN system consisting of 62.3 wt. % of CN and 31.7 wt. % of nematic E7, on concentration of BaTiO3 NPs.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-e86e29b0-7848-4532-a388-ebce289696ca.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-8611bb57-13dd-43f7-ae1e-5d5ffad70612.jpg)

Figure 12 shows the dependence of temperature Iso - BPs, Iso - N  and BPs - N * * transitions on concentration of CN of the mixtures doped by 0.5 wt. % of BaTiO3 NPs. As in case of the ISP mixtures containing COC, doping by 0.5 wt. % of BaTiO3 NPs the increase of the deviation from linear dependence T Iso ( C ) is observed.

In  comparison  with  mixtures  having  no  NPs  (Figure  9)  the  presence  of  NPs leads to the broadening of temperature range of BPs, which is the reason of sufficient increase  in  the  deviation  from  linear  dependence  both  on  heating  and  cooling  occurs (Figure 13).

Figure  13.  Dependence  of  the  temperature  of  transitions  Iso  -  BPs  (blue  squares symbols) and BPs - N * (red triangles symbols) E7-CN systems on concentration of CN during  (a)  heating  (solid  symbols)  and  (b)  cooling  (opened  symbols).  ISP  mixtures consisting of certain concentration ratio between CN and E7 and additionally doped by 0.5 wt. % BaTiO3 NPs. The studied E7-CN system contains 62.3 wt. % of CN and 31.7 wt. % of nematic E7. The linear dependence T C ( ) is shown by solid magenta line.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-a6e1d017-6321-467e-a8af-5e53471c30f9.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-cb06b457-313e-450f-bcdd-9b102024938b.jpg)

## 3.5 Experimental study of ISP mixtures based on COC and Ntb-forming mixture

In this section Ntb-COC systems containing certain concentration of COC in the Ntb-forming mixture will be considered to make a comparison between the behavior of conventional  4-cyanobiphenyls  and  bis(4-cyanobiphenyl-4′-yl)  alkanes  (CBnCB)  with odd  n  values  under  similar  conditions.  We  will  use  the  Ntb-forming  mixture  recently described in detail  elsewhere,  [53,54]  which  consists  of  two  nematic  dimers  CB7CB, CB6OCB  and  nematic  5CB  in  the  weight  ratio  39:19:42,  respectively.  Here,  the temperature  of  Iso  transition  as  function  of  COC  concentration  ( C COC)  attracted  the main attention.

It is also important to note that at certain concentration range of COC, which is approximately  from  19  to  90  wt.  %,  these  Ntb-COC  systems  are  in  a  specific  state characterised by two separated phases (Figure 14). Each of these phases characterised a separated branch of the phase transitions. Speaking of the transition to Iso, then Figure 14 shows the Iso phase transitions for both high temperature (opened black circles) and low temperature (opened green squares) branch of the phase transitions.

Taking into account the temperatures of the phase transitions for the Ntb [53] we can  conclude  that  the  high  temperature  branch  (Iso1)  corresponds  to  the  Iso  phase transition  of  Ntb-forming  mixture.  Then  the  low  temperature  branch  (Iso2)  can  be attributed to the phase transition of the nematic 5CB. [9]

Figure 14. The dependence of temperature of the transition to Iso for systems containing COC and the Ntb-forming mixture on concentration of COC. Two branches of Iso phase transition at high (opened black circles) and low (opened green squares) temperature are observed  within  concentration  range  from  19  to  90  wt.  %.  The  linear  dependence T Iso ( C COC) is shown by solid blue line.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-84eb9f36-e919-46d0-8201-3ee836a8b301.jpg)

The linear dependence of the T Iso ( C COC) is shown by the solid blue line (Figure 14).  The  deviation  from  linear  dependence T Iso ( C COC)  is  observed  for  the  Ntb-COC systems, containing COC within concentration range from 19 to 90 wt. % for which the presence of two branches of phase transitions is observed. For this concentration range the appearance of SA was also observed (Figure 15(d)).

Figure 15 shows the sequential textures of phase transitions on cooling for the Ntb-COC system containing COC and Ntb-forming mixture in weight ratio 1:1. There exist two  separated phase transitions for this complex  mixture.  The  sequential independent phase transitions, namely Iso-BPs/N -SA are observed. *

Figure  15.  The  sequential  textures  of  phase  transitions  on  cooling  for  the  Ntb-COC system, containing 50 wt. % of COC and 50 wt. % of Ntb-forming mixture: (a) Iso at 78.2 °C; (b) the appearance of bubble texture (N * 1) of the high temperature branch and Iso * 2  of  the  low  temperature  branch  at  71.8  °C;  (c)  N * 1  and  N * 2  at  30  °C;  (d)  the appearance of SA1 of the high temperature branch and N * 2 of the low temperature branch at  20  °C.  The  Ntb-forming  mixture  consists  of  two  nematic  liquid  crystal  dimers CB7CB, CB6OCB and nematic 5CB in the weight ratio 39:19:42, respectively.

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-065364e3-655c-4e1d-880a-ac56befbfa3f.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-966da328-1501-4bb7-ab16-7785c174006b.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-56738d7f-0de3-4758-9a44-dcb31b02d1de.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/2408.00650v1-figure-e11b8da7-0d76-4465-9fbf-e2f1f8e41658.jpg)

## Conclusions

Our idea was to study peculiar  features  of  phase  transitions  in  liquid  crystal  systems based  on  nematics  and  cholesterol  esters  as  a  peculiar  type  of  chiral  dopants.  In particular,  we  used  both  conventional  nematic  mixtures  like  E7  and  an  Ntb-forming mixture  comprising  CB7CB,  CB6OCB  and  5CB,  as  well  as  smectogenic  cholesteryl oleyl carbonate (COC) and cholesteryl nonanoate (CN).

The  E7-COC  systems  in  the  concentration  range  of  ~  25  -  80  wt.  %  COC showed a pronounced increase in the SA - N  transition temperature. This effect, which * can be considered as a sort of induced smectic phase (ISP) formation, was noticeably stronger  than  that  observed  earlier  with  5CB,  but  it  nearly  vanished  with  CN,  which supported  the  molecular  packing  mechanism  of  ISP  formation.  As  an  accompanying effect, it was found that such ISP mixtures showed a certain deviation from linearity of the  concentration  dependence  of  temperature  Iso  and  the  appearance  of  the  BPs,  the concentration range of which clearly correlated with the ISP formation.

The adding of the NPs, in particular, ferroelectric BaTiO3 NPs, to the ISP has led to an increase of the deviation from  linear dependence T Iso ( C ) caused  by  the stabilisation of BPs ( i.e. broadening of the temperature range of BPs).

In mixtures based on COC and Ntb-forming nematic, no induced smectics were observed, but they were characterised by two branches of the Iso transitions at higher and  lower  temperatures.  In  this  case  the  deviation  from  linear  dependence  of  the temperature of Iso transition on concentration of the chiral component is also observed.

## References:

- [1]. Park JW, Bak CS, Labes MM. Effects of molecular complexing on the properties of binary nematic liquid crystal mixtures. J Am Chem Soc. 1975; 97 (15): 43984400. DOI:10.1021/ja00848a045.
- [2]. Engelen B, Heppke G, Hopf R at al. Induced smectic phases. Ann Phys. 1978; 3: 403-407. DOI:10.1051/anphys/197803030403.
- [3]. Yu LJ,  Labes  MM.  Induced  smectic  mesomorphism  in  mixtures  of p -cyanop' -pentylbiphenyl  and p -pentylbenzoic  acid.  Mol  Cryst  Liq  Cryst.  1979;  54:  1-8. DOI:10.1080/00268947908084844.
- [4]. Waclawek W, Dabrowski R, Domagala A. On the intermolecular forces operating in induced smectics. Mol Cryst Liq Cryst. 1982; 84(1): 255-265. DOI:10.1080/00268948208072145.
- [5]. Dąbrowski R, Witkiewicz Z, Stolarzowa Z. Dwuskładnikowe układy ciekłokrystaliczne o zachowaniu nieaddytywnym, indukowane fazy smektyczne. Biul Wojsk Akad Techn. 1982; 31 (8): 125-149.
- [6]. Huang TM, McCreary K, Garg S et al. Induced smectic phases in phase diagrams of binary nematic liquid crystal mixtures. J Chem Phys. 2011; 134: 124508-1-10. DOI:10.1063/1.3567100.
- [7]. Sugisawa  S,  Tabe  Y.  Induced  smectic  phases  of  stoichiometric  liquid  crystal mixtures. Soft Matter. 2016; 12: 3103-3109. DOI:10.1039/c6sm00038j.
- [8]. Knežević A, Dokli I, Sapunar M et al. Induced smectic phase in binary mixtures of twist-bend nematogens. Belstein J Nanotechnol. 2018 ; 9: 1297-1307. DOI:10.3762/bjnano.9.122
- [9]. Lebovka NI, Lisetski LN, Nesterenko MI et al. Anomalous selective reflection in cholesteryl oleyl carbonate - nematic 5CB mixtures and effects of their doping by single-walled carbon nanotubes. Liq Cryst. 2013; 40 (7): 968-975. DOI:10.1080/02678292.2013.786796.
- [10]. Meiboom S, Sammon M. Blue phase of cholesteryl nonanoate. Phys Rev A. 1981; 24 (1): 468-475.
- [11]. Brazovskii SA, Dmitriev SG. Phase transitions in cholesteric liquid crystals. Sov. Phys. JETP. 1976; 42 (3): 497-502.
- [12]. Brazovskii SA, Filev VM. Critical phenomena in cholesteric liquid crystals. Sov Phys JETP. 1978; 48 (3): 573-578.
- [13]. Meiboom  S,  Sethna  JP,  Anderson  PW  et  al.  Theory  of  the  blue  phase  of cholesteric liquid crystals. Phys Rev Lett. 1981; 46 (18): 1216-1219.
- [14]. Wright  DC,  Mermin  ND.  Crystalline  liquids:  the  blue  phases.  Rev  Mod  Phys. 1989; 61 (2): 385-432.
- [15]. Khoo  IC,  Chen  CW,  Ho  TJ.  High  efficiency  holographic  Bragg  grating  with optically prolonged memory. Sci Rep. 2016; 6 (1): 36148-1-9.
- [16]. Jau HC, Lin YT, Li CC et al. Optically rewritable dynamic phase grating based on blue-phase-templated  azobenzene  liquid  crystal.  Opt  Express.  2019;  27  (8): 10580-10585.
- [17]. Choi HJ, Bae JH, Bae S, et al. Development of liquid crystal laser using a simple cubic liquid crystalline blue phase platform. RSC Adv. 2019; 9; 32922-32927.
- [18]. Dou H, Wang L, Chu F et al. A blue phase liquid crystal Fresnel lens with large transverse electric field component. Liq Cryst. 2020; 48 (5): 607-615.
- [19]. Cho S, Ozaki M. Blue phase liquid crystals with tailored crystal orientation for photonic applications. Symmetry. 2021; 13: 1584-1-14.
- [20]. Schlafmann KR, White TJ. Retention and deformation of the blue phases in liquid crystalline  elastomers.  Nat  Commun. 2021; 12:  4916-1-9. DOI:10.1038/s41467021-25112-6.
- [21]. Gurboga  B,  Kemiklioglu  E.  Optical  sensing  of  organic  vapor  using  blue  phase liquid crystals. Liq Cryst. 2022; 49 (11): 1428-1435. DOI:10.1080/02678292.2022.2038294.
- [22]. Gvozdovskyy IA, Kachurak YM, Vashchenko PV et al. Liquid crystal sensors for detection of volatile organic compounds: comparative effects of vapor absorption and temperature on the phase state of the sensor material. Funct Mater  2023; 30 . (2): 303-308. DOI:10.15407/fm30.02.303.
- [23]. Rahman MDA, Said SM, Balamurugan S. Blue phase liquid crystals: strategies for phase stabilization and device development. Sci Technol Adv Mater. 2015; 16: 033501-1-21.
- [24]. Dierking I. Textures of liquid crystals. Wiley-VCH, Verlag GmbH&amp;Co. KGaA: Weinheim; 2003.
- [25]. Dierking I, Flatley A, Greenhalgh D. Voronoi patterns in liquid crystal textures . J Mol Liq. 2021; 335: 116553-1-8. DOI:10.1016/j.molliq.2021.116553.
- [26]. Dierking  I,  Flatley  A,  Greenhalgh  D.  Can  liquid  crystal  blue  phase  textures  be described by Voronoi tessellations? Liq Cryst. 2021; 48(5): 689-698. DOI:10.1080/02678292.2020.1811411.
- [27]. Voronoi  GF.  Nouvelles  applications  des  paramèter  continues  à  la  théorie  de formes  quadratiques.  Deuxième  mémoire.  Recherches  sur  les  parallélloèdres primitifs. J für die reine und angewandte Mathematik. 1908; 133: 97-178.
- [28]. Fukuda I, Žumer S. Lattice orientation of cholesteric blue phases in contact with surfaces  enforcing  unidirectional  planar  anchoring.  Phys  Rev  Res.  2020;  2: 033407-1-11. DOI:10.1103/PhysRevResearch.2.033407.
- [29]. Gleeson  HF,  Miller  RJ,  Tian  l  et  al.  Liquid  crystal  blue  phases:  stability,  field effects and alignment. Liq Cryst. 2015; 42(5-6): 760-771. DOI:10.1080/02678292.2014.1002821
- [30]. Takahashi M, Ohkawa T, Yoshida H, et al. Orientation of liquid crystalline blue phases on inidirectionally orienting surfaces. J Phys D Appl Phys. 2018; 51(10): 104003-1-8. DOI: 10.1088/1361-6463/aaaa4b.
- [31]. Otón E, Morawiak P, Gaładyk K et al.  Fast self-assembly of macroscopic blue phase 3D photonic crystals. Opt Express. 2020; 28 (12): 18202-18211. DOI:10.1364/OE.393197.
- [32]. Li  X,  Martínez-González  JA,  Hernández-Ortiz  JP  et  al.  Mesoscale  martensitic transformation in single crystals of topological defects. Proc Natl Acad Sci USA. 2017; 114(38):10011-10016. DOI:10.1073/pnas.1711207114.
- [33]. Li  X,  Park  K,  Guzmán  O,  et  al.  Nucleation  and  growth  of  blue  phase  liquid crystals on chemically-patterned surfaces: a surface anchoring assisted blue phase correlation length. Mol Syst Des Eng. 2021; 6(7): 534-544. DOI:10.1039/d1me00044f.
- [34]. Nakajima K, Tsukamoto Y, Mitsuhashi S, et al. Frustrated lattice orientation of cholesteric  blue  phase  II  induced  by  micro-patterned  surface  alignment.  Appl Phys Express. 2022; 15(7):071007-1-4. DOI:10.35848/1882-0786/ac75aa
- [35]. Kossel  W,  Loeck  V,  Voges  H.  Die  Richtungsverteilung  der  in  einem  Kristall entstandenen charakteristischen Röntgenstrahlung. Z Physik. 1935; 94: 139-144. DOI:https://doi.org/10.1007/BF01330803.
- [36]. Jerome  B,  Pieranski  P.  Kossel  diagrams  of  blue  phases.  Liq  Cryst.  1989;  5(3): 799-812.
- [37]. Xiang  J,  Lavrentovich  OD.  Blue-phase-polymer-templated  nematic  with  submillisecond  broad-temperature  range  electro-optic  switching.  Appl  Phys  Lett. 2013; 103: 051112-1-4. DOI:10.1063/1.4817724.
- [38]. Abberley  JP,  Killah  R,  Walker  R  et  al.  Heliconical  smectic  phases  formed  by achiral molecules. Nat Commun. 2018; 9(1): 228-1-9. DOI:10.1038/s41467-01702626-6.
- [39]. Salamończyk  M,  Vaupotič  N,  Pociecha  D  et  al.  Structure  of  nanoscale-pitch helical phases: blue phase and twist-bend nematic phase resolved by resonant soft X-ray scattering. Soft Matter. 2017; 13: 6694-6699. DOI:10.1039/c7sm00967d
- [40]. Huang H, Li J, Du A et al. Bent-structure liquid crystalline dimers containing a cholesteryl group exhibiting blue phases. Cryst Growth Des. 2022; 22 (12): 74787490. DOI:10.1021/acs.cgd.2c01045.
- [41]. Dierking  I,  Blenkhorn  W,  Credland  E  et  al.  Stabilizing  liquid  crystalline  blue phases. Soft Matter. 2012; 8: 4355-4362.
- [42]. Cordoyiannis  G,  Losada-Perez  P,  Shekhar  Pati  Tripathi  C  et  al.  Blue  phase  III widening in CE6-dispersed surface-functionalised CdSe nanoparticles. Liq Cryst. 2010; 37: 1419-1426.
- [43]. Kikuchi H, Yokota M, Hisakado Y et al. Polymer-stabilized liquid  crystal  blue phases. Nat Mater. 2002; 1 (1): 64-68. DOI:10.1038/nmat712.
- [44]. Coles H, Pivnenko M. Liquid crystal 'blue phases' with a wide temperature range. Nature. 2005; 436: 997-1000. DOI:10.1038/nature03932.
- [45]. Fukushima S, Tokunaga K, Morishita T et al. Polymer-stabilized blue phase and its  application  to  a  1.5  µm  band  wavelength  selective  filter.  Crystals.  2021;  11: 1017-1-8. DOI:10.3390/cryst11091017.
- [46]. Wang M, Song H, Wu C et al. Synthesis of thiophene-based derivatives and the effects of their molecular structure on the mesomorphic behavior and temperature range of liquid-crystalline blue phases. Crystals. 2023; 13 (6): 916-1-13. DOI:10.3390/cryst13060916.
- [47]. Yoshizawa  A,  Sato  M,  Rokunohe  J.  A  blue  phase  observed  for  a  novel  chiral compound possessing molecular biaxiality. J Mater Chem. 2005; 15 (32): 32853290. DOI:10.1039/B506167A.
- [48]. Guo J,  Shi  Y,  Han  X  et  al.  Stabilizing  blue  phases  of  a  simple  cyanobiphenyl compound by addition of achiral mesogen monomer with a branched end group and chiral hydrogen-bonded assemblies. J Mater Chem. C. 2013; 1: 947-957.
- [49]. Gvozdovskyy I. 'Blue phases' of highly chiral thermotropic liquid crystals with a wide range of near-room temperature. Liq Cryst. 2015; 42 (10): 1391-1404. DOI: 10.1080/02678292.2015.1053001.
- [50]. Lavrič M, Tzitzios V, Kralj S et al. The effect of graphene on liquid-crystalline blue phase. Appl Phys Lett. 2013; 103: 143116-1-4. DOI:10.1063/1.4824424.
- [51]. Wang L, He W, Xiao X et al. Low voltage and hysteresis-free blue phase liquid crystal  dispersed  by  ferroelectric  nanoparticles.  J  Mater  Chem   2021;  22:  1929-. 19633. DOI:10.1039/c2jm34013e.
- [52]. Licristal brochure, Merck Liquid crystals, 1994.
- [53]. Chornous V, Grozav A, Vovk M et al. Oblique helicoidal state of the twist-bend nematic  doped  by  chiral  azo-compound.  Liq  Cryst   2023;  50  (6):  1046-1058. . DOI:10.1080/02678292.2023.2200267.
- [54]. Bogatyryova H, Chornous V, Lisetski L et al. Bragg diffraction of higher orders on oblique helicoidal liquid crystal structures. Liq Cryst. 2024 (doi:10.1080/02678292.2024.2361484).
- [55]. Peterson DA, Gao M, Kim YK et al. Understanding the twist-bend nematic phase: the characterisation of 1-(4-cyanobiphenyl-4′-yloxy)-6-(4-cyanobiphenyl-4′yl)hexane (CB6OCB) and comparison with CB7CB. Soft Matter. 2016; 12: 68276840. DOI:10.1039/C6SM00537C
- [56]. Walker R,  Pociecha  D,  Storey  JMD  et  al.  The  chiral  twist-bend  nematic  phase (NTB). Chem Eur J  2019; 25 (58); 13329-13335. DOI:10.1002/chem.201903014. .
- [57]. Paterson  DA,  Abberley  JP,  Harrison  WTA  et  al.  Cyanobiphenyl-based  liquid crystal  dimers  and  the  twist-bend  nematic  phase.  Liq  Cryst.  2017;  44  (1):  127146. DOI:10.1080/02678292.2016.1274293.
- [58]. Davis GJ, Porter RS, Barral II EM. An intercomparison of temperatures and heats of transition for esters of cholesterol. Mol Cryst Liq Cryst. 1970; 11(4): 319-330. DOI:10.1080/15421407008083524.
- [59]. McMillan WL. X-ray scattering from liquid crystals. I. Cholesteryl nonanoate and myristate. Phys Rev A. 1972; 6(2): 936-947. DOI:10.1103/PhysRevA.6.936.
- [60]. HD MicroSystems Product bulletin PI2525, PI2555 and PI2574; 2012 Nov.
- [61]. Yang  FZ,  Cheng  HF,  Gao  HJ  et  al.  Technique  for  characterizing  azimuthal anchoring of twisted nematic liquid crystals using half-leaky guided modes. J Opt Soc Am B. 2001; 18 (7): 994-1002. DOI:10.1364/JOSAB.18.000994.
- [62]. De Gennes PG, Prost J. The physics of liquid crystals. Oxford: Clarendon Press; 1993.
- [63]. Nesterkina M, Vashchenko O, Vashchenko P et al. Thermoresponsive cholesteric liquid-crystal  systems  doped  with  terpenoids  as  drug  delivery  systems  for  skin applications. Eur J Pharm Biopharm. 2023; 191: 139-149. DOI: 10.1016/j.ejpb.2023.09.002
- [64]. Otón  E,  Yoshida  H,  Morawiak  P  et  al.  Orientation  control  of  ideal  blue  phase photonic crystals. Sci Rep. 2020; 10: 10148-1-8. DOI:10.1038/s41598-020-67836.
- [65]. Duarte EL, Palangana AJ, Itri R, et al. Smectic A - cholesteric liquid crystal phase transition: a density study. Eur Phys J B. 1998; 5(4): 835-838. DOI:10.1007/s100510050509.
Natalia A. Kasian Longin N. Lisetski Serhii E. Ivanchenko Vitalii O. Chornous Halyna V. Bogatyryova Igor A. Gvozdovskyy
Induced smectic ordering and blue phase formation in mixtures of cyanobiphenyls and cholesterol esters
It has been found that in mixtures of nematic E7 and smectogenic cholesteryl
oleyl carbonate (COC) the S$_A$-N* transition temperature is substantially (by
~20 K) increased, as compared with pure COC, at E7 concentrations around ~40%.
Within the same concentration range, the isotropic transition is preceded by
formation of blue phase, with its maximum width of ~3.5 K clearly correlated to
the increased thermal stability of the S$_A$ phase. With other cholesterol
esters or cyanobiphenyls (cholesteryl nonanoate, 5CB), this effect was either
much weaker or not observed. No enhancement of smectic phase was noted when E7
was replaced by N$_{tb}$-forming nematic mixture based on CB7CB with two
cyanobiphenyl moieties. Selective Bragg reflection of light (BRL) spectra were
measured in all three temperature regions, including the unwinding of the
cholesteric helix on cooling towards S$_A$ phase and characteristic selective
BRL changes in the blue phase. In the latter case, the measured
{\lambda}$_{max}$ values were dependent both on the helical twisting power in
the cholesteric phase and on the lattice size and orientation in the blue
phase. Also considered were the effects of ferroelectric BaTiO$_3$
nanoparticles accumulated at disclination lines upon the blue phase thermal
stability.